Abstract
Superconductivity in low carrier density metals challenges the conventional electronphonon theory due to the absence of retardation required to overcome Coulomb repulsion. Here we demonstrate that pairing mediated by energy fluctuations, ubiquitously present close to continuous phase transitions, occurs in dilute quantum critical polar metals and results in a domelike dependence of the superconducting T_{c} on carrier density, characteristic of nonBCS superconductors. In quantum critical polar metals, the Coulomb repulsion is heavily screened, while the critical transverse optical phonons decouple from the electron charge. In the resulting vacuum, longrange attractive interactions emerge from the energy fluctuations of the critical phonons, resembling the gravitational interactions of a chargeless dark matter universe. Our estimates show that this mechanism may explain the critical temperatures observed in doped SrTiO_{3}. We provide predictions for the enhancement of superconductivity near polar quantum criticality in two and threedimensional materials that can be used to test our theory.
Similar content being viewed by others
Introduction
Superconductivity exemplifies the dramatic effects of interactions in manybody quantum systems^{1}. In conventional superconductors, electrons exploit the electronphonon interaction to overcome the Coulomb repulsion^{2,3} by producing a highly retarded attraction that pairs electrons. This process requires a large ratio between the Fermi and Debye energies E_{F}/ω_{D} > > 1^{4}. A challenge to this mechanism is posed by superconductivity in low carrier density metals near polar quantum critical points (QCPs). Such materials, typified by doped SrTiO_{3} (STO)^{5}, exhibit bulk superconductivity down to carrier densities of order 10^{19} cm^{−3}, where the relevant phonon frequency exceeds the Fermi energy^{5} by orders of magnitude. Yet despite this inversion of energy scales, experiments^{6,7} indicate a conventional swave condensate, with a ratio of gap to transition temperature 2Δ/T_{c} ≈ 3.5 in agreement with BCS theory^{7}.
Several theories have been advanced to explain superconductivity in polar metals using the conventional electronphonon interaction^{8} and its extension to include plasmons^{9,10,11,12}. Recently, it has been proposed that the underlying polar quantum criticality is a key driver in the pairing^{13,14,15,16}. However, this appealing idea encounters a difficulty, for the critical modes of a polar QCP are transverse optical (TO) phonons for which the conventional electronphonon coupling vanishes at low momenta^{17,18,19}. Alternative phonon coupling mechanisms requiring spinorbit coupling or multiband effects^{20,21,22} (such as Dirac points^{23,24}) have also been examined and possible superconductivity^{23,25,26} has been discussed.
We reassess superconductivity in quantum critical polar metals guided by two key observations: first, that the strong ionic screening associated with the enhanced dielectric constant severely weakens the electronic Coulomb interaction (Fig. 1a); second, that in the absence of strong spinorbit coupling the transverse optical phonon modes, decoupled from the electron charge, can be likened to dark matter, for like baryons in the cosmos, the electrons do not directly interact with the the intense background of zeropoint dipole fluctuations. Furthermore like dark matter, the presence of the TO modes is only revealed to the electrons via their stressenergy tensor. In particular, the electrons interact with the energy density of the TO phonons. We model this coupling by the Hamiltonian^{27,28,29}:
where ρ_{e}(x) = ψ^{†}(x)ψ(x) is the electron density, \(({\bf P}({{{{{{{\bf{x}}}}}}}}))^{2}\) is proportional to the energy density of the local polarization P and g is a coupling constant with the dimensions of volume. Microscopically, this interaction can be thought of as arising from the shortrange effects of the Coulomb force within a unit cell of the material. The presence of an additional charge at the conduction electron site modifies the potential profile for the ions. A local increase in the electron density attracts the surrounding positively charged ions, reducing the distance between them. This causes the local “effective spring constant” of the phonons to rise in regions of high electon density. The natural units for this interaction are therefore atomic ones, i.e. unit cell volume, and should not be extremely different between different materials.
This coupling suppresses the zeropoint fluctuations of the polarization in the vicinity of electrons, which in turn lowers the chemical potential of nearby electrons (Fig. 1b), creating an attractive potential well. To lowest order, the resulting attractive potential is described by the virtual exchange of pairs of TO phonons (see Supplementary Information for details), allowing us to link these ideas to two recent observations: first, that twophonon exchange appears to drive the anomalous “hightemperature” T^{2} resistivity of polar metals^{29,30}, and second that twophonon processes may drive superconductivity^{31}, reviving an old idea^{27}. At the same time, energy fluctuations are present in the vicinity of all continuous phase transitions, implying that their coupling to electrons must be relevant for a broad range of systems.
Here we study the consequences of the coupling to energy fluctuations of the order parameter (1) in quantum critical polar metals. We find that polar quantum criticality results in longrange “gravitational" interactions that mediate attraction between the electrons in an electromagnetically neutral background. This attraction overcomes the critically screened Coulomb repulsion and leads to superconductivity at extremely low densities. With increasing carrier concentration, the longrange character of the attraction is concealed due to shorter distances between electrons, leading to a domelike superconducting region in the phase diagram. The application of our theory to SrTiO_{3} shows good agreement with the observed magnitude and doping dependence of T_{c}. We predict that the impact of this novel mechanism will be considerably enhanced in twodimensional quantum critical polar systems.
Results
Our theory is built on an isotropic model for the polar metal, with an action S[ψ^{†}, ψ, P] = S_{e} + S_{C} + S_{En}. Here S_{En} = ∫dτH_{En} is the energy fluctuation term (1), \({S}_{e}={\sum }_{k}{\psi }_{k}^{{{{\dagger}}} }({\epsilon }_{\bf k}i{\varepsilon }_{n}){\psi }_{k}\), is the electronic action, in terms of the Fourier transformed electron field ψ_{k}, where k ≡ (iε_{n}, k) is a fourvector containing the Matsubara frequency ε_{n} = (2n + 1)πT and wavevector k. The action of electrostatic interactions and the polar phonons is given by
where the total charge densities eρ_{e} − ∇ ⋅ P and q ≡ (iω_{n}, q), where ω_{n} = 2nπT. ε_{1} is the bare dielectric constant, Ω_{0} is the ionic plasma frequency, ω_{T0} is the transverse optical mode frequency and c_{s} is the speed of the transverse optical mode. \({\omega }_{T0}^{2}\) vanishes at the QCP. The Gaussian coefficients of the polarization, \({\delta }^{2}{S}_{C}/\delta {P}_{a}(q)\delta {P}_{b}(q)={D}_{ab}^{1}(q)\) in (2), separate into transverse and longitudinal components
where \({D}_{L,T}^{1}(q)=({\omega }_{n}^{2}+{\omega }_{T0,L0}^{2}+{c}_{s}^{2}{q}^{2})/{\varepsilon }_{0}{{{\Omega }}}_{0}^{2}\) are the inverse longitudinal and transverse phonon propagators. The longitudinal optical mode frequency \({\omega }_{L0}^{2}={\omega }_{T0}^{2}+{{{\Omega }}}_{0}^{2}/{\varepsilon }_{1}\) is shifted upwards by the Coulomb interaction.
We first consider the case where g = 0. Integrating over the longitudinal modes, we find that the Coulomb interaction becomes
where
is the renormalized dielectric constant and \({P}_{a}^{T}(q)=({\delta }_{ab}{\hat{q}}_{a}{\hat{q}}_{b}){P}_{b}(q)\) are the transverse components of the polarization. Most importantly, in action (4) the quantum critical transverse polar modes are entirely decoupled from the electronic degrees of freedom, motivating the dark matter analogy.
Normally, low carrier density metals are considered strongly interacting, for the ratio of Coulomb to kinetic energy, determined by r_{s} = 1/(k_{F}a_{B}), where \({k}_{F} \sim {n}_{e}^{1/3}\) is the Fermi momentum and \({a}_{B}=\frac{4\pi \varepsilon {\hslash }^{2}}{{m}^{*}{e}^{2}}\) the Bohr radius, is very large at low densities. However, in a quantum critical polar metal, the large upward renormalization of the dielectric constant, Eq. (5), severely suppresses the interaction between the electrons. Indeed, the dielectric constant at the relevant electronic scales at low densities is \(\varepsilon \sim \varepsilon ({{{{{{{\bf{q}}}}}}}},\,{\omega }_{n}){}_{q=2{k}_{F},{\omega }_{n}={E}_{F}}\approx \frac{{{{\Omega }}}_{0}^{2}}{{(2{c}_{s}{k}_{F})}^{2}}\gg 1\) at the polar QCP, leading to r_{s} ≪ 1. Furthermore, the electronic corrections to the dielectric constant, given in random phase approximation (RPA) by \(\delta {\varepsilon }_{RPA}=\frac{{e}^{2}}{{q}^{2}{\varepsilon }_{0}}{{{\Pi }}}_{e}({{{{{{{\bf{q}}}}}}}},\,{\omega }_{n})\), where Π_{e}(q, ω_{n}) is the dynamical susceptibility (Lindhardt function) of the electron gas, can be neglected. Indeed, \(\frac{\delta {\varepsilon }_{RPA}}{\varepsilon }{}_{q=2{k}_{F},{\omega }_{n}={E}_{F}} \sim {r}_{s}\,\ll\, 1\).
The regime considered here lies in stark contrast to the conventional case, where the relevant longitudinal phonon frequency is much smaller than E_{F}. In this regime, the electronic plasmon appears at low energies v_{F}q ≪ ω_{n}. However, its contribution to pairing is suppressed by the factor ε^{−1}^{10}. Thus, in what follows we neglect this possibility, approximating the electron dynamical susceptibility by its long wavelength, lowfrequency limit as in (5).
We next consider the effect of turning on the coupling to energy fluctuations in (1). The presence of a finite electron density n_{e} = 〈ρ_{e}(x)〉 leads to a shift in the phonon frequency:
which naturally explains the suppression of the polar state by charge doping, universally observed in polar metals^{15,32}. Though this effect only shifts the position of the polar QCP, it must be included when considering properties as a function of electronic density. For example a system that is initially polar with \({\omega }_{T0}^{2} \, < \, 0\) and g > 0 will have a polar QCP at a finite density, as is observed in CaSr substituted SrTiO_{3}^{15}.
The coupling of the energy fluctuations to the electron density fluctuations δρ_{e}(x) = ρ_{e}(x) − n_{e}, cannot be integrated out exactly. Interactions with critical fluctuations near QCPs can be relevant perturbations in a scaling sense^{33}, destabilizing the Fermi liquid ground state already at weak coupling^{33}. In our case, however, the interaction Eq. (1) preserves the Fermi liquid. Assuming the dynamical critical exponent z = 1 and taking the scaling dimension of momentum [q] = 1, one obtains [g] = 2 − d, irrelevant in 3D (see Supplementary Information for details), implying that the system remains a Fermi liquid even at the QCP (whereas in the known cases of nonFermi liquid behavior the interaction remains at least marginal^{33}). Thus, we can consider its effects perturbatively for weak coupling. Integrating out the field P(x) to lowest order in g, we obtain an effective interaction between electrons:
where
is recognized to be an attractive densitydensity interaction resulting from twophonon exchange, Fig. 1b. At criticality, the contribution to Eq. (8) of the transverse modes stems from their propagator
leading to an attractive longrange interaction of the form
where \(\alpha={\left(\frac{g{\varepsilon }_{0}{{{\Omega }}}_{0}^{2}}{2{\pi }^{2}{c}_{s}}\right)}^{2}\), which plays the role of an emergent “gravitational” attraction between electrons at a polar QCP. These interactions also act on the TO phonons via the quartic term in their action^{33,34} (see Supplementary Information for details). In what follows we will not consider this effects, assuming the relevant momenta and energies to be always larger than the critical region in the energymomentum space set by the phononphonon interactions.
Away from criticality, (10) is valid for spacetime separations smaller than the correlation length ξ = c_{s}/ω_{T}. The qualitative form of the interaction at finite momentum and frequency transfer, relevant for pairing, is obtained by a Fourier transform of this expression with a longdistance cutoff ξ
where \({\omega }_{q}=\sqrt{{\omega }_{n}^{2}+{c}_{s}^{2}{{{{{{{{\bf{q}}}}}}}}}^{2}}\). The characteristic electronic momentum and energy transfer scales are q ~ k_{F} ~ n^{1/3} and ω_{n} ~ E_{F} ~ n^{2/3}, respectively, resulting in ∣q∣^{−1} ~ n^{−1/3}, c_{s}/∣ω_{n}∣ ~ n^{−2/3}. Furthermore, following (6), a finite electron density leads to a finite correlation length of the order ξ ~ n^{−1/2}. Consequently the interaction character changes with density, and can be described by an effective interaction \({V}_{En}^{Pair}({{{{{{{\bf{x}}}}}}}},\tau )\) obtained by inverse Fourier transforming the final result of Eq. (11) (Fig. 2). For a low density polar metal that is critical at zero doping (ω_{T0} = 0) one expects the interaction to be cut off at the Fermi momentum k_{F}, while being essentially independent of frequency, since E_{F}/c_{s} ≪ k_{F}. This is identical to an instantaneous repulsion, nonlocal in real space (Fig. 2, middle):
in analogy with the instantaneous Newtonian gravity emerging at low energies from the “relativistic" interaction (10). This case is also realized for a system away from a QCP (ω_{T0} > 0) at intermediate densities (c_{s}k_{F} ≫ ω_{T}(n_{e}), E_{F}, see Fig. 2). In the high density limit, the frequencydependence of the interaction can be no longer ignored and it is suppressed for frequencies beyond c_{s}k_{F}, qualitatively similar to a usual phononmediated attraction (Fig. 2, rightmost region). Finally, if ω_{T}(n_{e}) ≫ E_{F}, c_{s}k_{F} (leftmost region of Fig. 2), which can be realized away from the QCP at the lowest densities, the interaction \({V}_{En}^{Pair}({{{{{{{\bf{x}}}}}}}},\,\tau )\) reduces to an instantaneous local attraction.
A more detailed calculation of the interaction potential (see Supplementary Information for details) yields
where Ω_{T} is the upper cutoff for the optical phonon frequency throughout the Brillouin zone. Here it is important to note, that since the integral is logarithmically divergent, large momenta of the order of the Brillouin zone size contribute significantly. At such momenta, the dispersion is expected to deviate from simply quadratic. Thus in practical calculations, an average value of c_{s} should be used in the prefactor of (13), which we take in the spirit of Debye approximation to be equal to \({\overline{c}}_{s}={{{\Omega }}}_{T}/({(6{\pi }^{2})}^{1/3}/{a}_{0})\). We remark that the contribution of the longitudinal modes to the induced interaction can be shown to be negligible in the critical lowdensity regime, where Ω_{T} ≫ ω_{T}(n_{e}), c_{s}k_{F} and \(\frac{{{{\Omega }}}_{0}^{2}}{{c}_{s}^{2}{k}_{F}{a}_{B}^{1}}\,\gg\, 1\) (see Supplementary Information for details).
Superconductivity at low densities
We now show that the attractive interaction mediated by the energy fluctuations always leads to superconductivity at low densities close to the polar QCP. In particular, the density is assumed to be in the middle regime of Fig. 2, i.e. E_{F}, ω_{T}(n_{e}) ≪ 2c_{s}k_{F}, allowing us to neglect ω_{n} in the interaction. Averaging the repulsive Coulomb ((4), (5)) and the attractive (13), interactions over the Fermi surface, i.e. \(\langle V(kk^{\prime} )\rangle={\langle V({k}_{F},{k}_{F},\theta )\rangle }_{\theta }\), we obtain (see Supplementary Information for details):
where \(N(0)=\frac{{k}_{F}{m}^{*}}{2{\pi }^{2}{\hslash }^{2}}\) is the density of states and \(\overline{\alpha }\) is equal to α with \({c}_{s}\to {\overline{c}}_{s}\). In deriving this we used that ω_{T} ~ (gn)^{1/2}, E_{F} ~ n^{2/3} ≪ c_{s}k_{F} ~ n^{1/3}. Most importantly, we find that at low enough doping the twophonon attraction inevitably overcomes the Coulomb repulsion due to the logarithmic enhancement of the former. In particular, the total interaction is attractive for densities below
where \(\gamma \sim 40\frac{{a}_{B}}{{a}_{0}}\frac{{E}_{h}{{{\Omega }}}_{T}^{5}}{{{{\Omega }}}_{0}^{6}}\) for \(g \sim {a}_{0}^{3}\). For strongly polar materials, Ω_{0} ≫ Ω_{T} and hence γ ≪ 1, so this restriction is unimportant. Moreover, from (14) the attractive part of the interaction behaves as \(\lambda \propto {k}_{F}\left\{\log ({{{\Omega }}}_{T}/(2{c}_{s}{k}_{F}))+1\right\}\), describing a domeshaped behavior of the attractive coupling constant peaked at k_{F} = Ω_{T}/2c_{s} corresponding to a density:
As the phonon dispersion flattens near the Brillouin zone edges, the average \({\overline{c}}_{s} \, < \, {c}_{s}\) so that \({n}_{max}{a}_{0}^{3}\,\ll\, 1\), corresponding to a dilute charge concentration below half filling. Finally, away from the QCP (i.e. ω_{T0} ≠ 0), the Coulomb screening is reduced, resulting in an additional repulsive term \(\sim 2\pi {e}^{2}{\omega }_{T}^{2}({n}_{e})/({{{\Omega }}}_{0}^{2}{k}_{F}^{2})\) (c.f. (5)). Due to its singular nature at k_{F} → 0 this sets a lower bound on the density \({n}_{min} \sim {\xi }^{3}{[\gamma /\log ({{{\Omega }}}_{T}/{\omega }_{T}({n}_{e}))]}^{3/2}/3{\pi }^{2}\) where the interaction is attractive. Therefore, both proximity to the QCP and sufficiently low densities are required to generate an attractive interaction.
Let us now discuss the critical temperatures of the resulting superconductor. At low densities, the interaction is essentially instantaneous (see Fig. 2). The critical temperature can then be found in the nonadiabatic weakcoupling limit to be T_{c} ≈ 0.28E_{F}e^{−1/λ} (which includes vertex corrections to the interaction)^{35,36}. Due to the exponential dependence on the coupling constant, one expects T_{c} to have a domelike shape with a maximum at n_{max} as in (16). The theory developed here also has important consequences for the dependence of T_{c} on external tuning parameters (e.g. pressure) in the vicinity of a polar QCP. Neglecting the residual Coulomb term in (14) and thus assuming the dominance of the energyfluctuation attraction, one obtains
For ω_{T}(n_{e}) ≫ c_{s}k_{F}, a singular dependence of T_{c} on tuning parameter near the QCP is observed. However, at intermediate densities (ω_{T}(n_{e}) ≪ c_{s}k_{F}, Fig. 2, middle panel), the coupling constant is almost independent of the TO phonon frequency, so the tuning sensitivity will be much weaker.
2D polar metals
Similar calculations can be performed in two dimensions. While at tree level, Eq. (1) is marginal, the corrections due to quartic interactions between phonons introduce an anomalous dimension to the energy fluctuations, reducing their momentumspace singularities^{37}, which allows to preserve the Fermi liquid in 2D (see Supplementary Information for details). We note that the anomalous dimension of the energy fluctuations makes them distinct from the perturbative twophonon processes in the 2D case at low momenta/frequencies. Indeed, the presence of an anomalous dimension indicates that the phonons are no longer welldefined quasiparticles^{33} so that the energy fluctuations can no longer be uniquely defined as a twophonon exchange. However, for momenta larger than a critical one (set by the phononphonon interactions), (11) is expected to be valid. The 2D Fourier transformation of expression (11) yields
 a stronger singularity than in 3D. In the limit c_{s}k_{F} ≫ ω_{T}(n_{e}) the terms due to LO phonon energy fluctuation also have to be included, being of the same order, but this does not change the qualitative form of the interaction (see Supplementary Information for details). Finally, the bare Coulomb repulsion in 2D is given by \(\frac{{e}^{2}}{2{\varepsilon }_{0}q}\). Screening with the polar mode and conduction electrons, however, reduces it to
where l_{0} is the 2D layer thickness.
Superconductivity in Doped SrTiO_{3}
We now apply these results to doped SrTiO_{3}. Figure 3a displays the doping dependence of T_{c} calculated using the parameters from the literature (see Supplementary Information for details) and taking the coupling g as a fitting parameter. The resulting value \(g/{a}_{0}^{3}\,\approx\, 0.68\) is comparable to ones obtained from fits to the T^{2} resistivity (\(g/{a}_{0}^{3}\,\approx\, 0.5\), note the factor of two in the definition of the coupling^{29}) and doping dependence of the TO phonon frequency (\(g/{a}_{0}^{3}\,\approx\, 0.56\) can be deduced from^{38}). We assume an effective oneband model with mass m^{*} = 4m_{e}. The Hall effect and quantum oscillation data^{39} indeed suggest that one of the three bands occupied in SrTiO_{3} contains the most carriers (by an order of magnitude) and has the largest effective mass, dominating the density of states. For the energy fluctuation interaction, Eq.(13), we assumed 2c_{s}k_{F} ≫ E_{F}, which holds in SrTiO_{3} for densities lower than 2.6 ⋅ 10^{19} cm^{−3}. As discussed before (see Fig. 2), this allows us to approximate the interactions with an instantaneous one. In this approximation, 2Δ/T_{c} takes the BCS value 3.52^{35,36}, in accord with STM experiments^{7}.
If the Coulomb repulsion (represented for intermediate densities by the second term in Eq. (14)) is neglected (gray dashed line in Fig. 3a) both the magnitude and the doping dependence of the critical temperature are in good agreement with experiment^{39,40} at all electron concentrations. The domelike shape of T_{c}(n_{e}) arises from the nonomonotonic dependence of the twophonon attractive coupling constant on density, initially rising with the density of states, subsequently decreasing as the lower energy cutoff c_{s}k_{F} grows. Importantly, the position of the T_{c} peak, n_{max} is approximately independent of the only free parameter of our theory, the coupling constant g  indeed, Eq. (16) yields n_{max} ≈ 5.5 ⋅ 10^{20} cm^{−3}, close to the actual value. Including the Coulomb repulsion (black line in Fig. 3a, see Supplementary Information for details), the results based on the instantaneous approximation do not agree as well with the experimental data for densities higher than 2.6 ⋅ 10^{19} cm^{−3}. Indeed, since in this regime E_{F} ≳ 2c_{s}k_{F}, frequency dependence of the interaction can be no longer ignored. Whilst a detailed analysis of the frequencydependent equations is beyond the scope of the current work, we observe that while the Coulomb repulsion strengthens as a function of frequency (see Eq. (5)), the attraction from energy fluctuations, Eq. (11), becomes weaker. Thus we expect that the interaction will change its sign as a function of frequency, allowing for an enhancement of the pairing via the effects of retardation^{2,3}. We note that a second superconducting dome has been observed at yet lower densities n_{e} ~ 10^{18} cm^{−3}^{41,42}; however, the Meissner effect is absent for this second dome^{5,42}. This suggests a highly inhomogeneous state likely affected by the nature of the dopants^{43}, effects that lie beyond the current model.
As discussed above, proximity to a polar QCP should enhance T_{c}, particularly at low densities. Such a correlation has been observed for the cases of oxygen isotope substitution^{14} as well as CaSr substitution^{15}, pressure^{11} or strain^{44,45}. In particular, the enhancement is observed to be more pronounced at low dopings^{15}, in qualitative agreement with the arguments given above, see also Fig. 3a, green dashed line. Note also, that in the polar phase close to the QCP the interaction (1) would still lead to pairing due to fluctuations of the order parameter amplitude around the equilibrium value.
Above we have mentioned, that critical effects for pairing should be emphasized in 2D systems. We propose that thin films of SrTiO_{3} may provide a platform to explore the predictions of the energy fluctuation theory. Figure 3b displays the predicted T_{c}, using T_{c} = 0.15E_{F}e^{−1/λ} for 2D instantaneous pairing (c_{s}k_{F} ≫ ω_{T}(n_{e}))^{36}), using coupling constants appropriate for a twolayer thick slab of SrTiO_{3}. Assuming that the electrons and phonons are in the lowest lateral quantization state, we obtain g_{2D} = g/(2a_{0}) (see Supplementary Information for details). The results show that an appreciable T_{c} is obtained at low densities. Furthermore, T_{c} is highly sensitive to the approach to criticality: a slight decrease of the TO phonon frequency leads to an enormous increase of T_{c}.
Discussion
New polar metals are being actively discovered^{46}; our theory suggests that suppression of the polar structural transition, for example by pressure^{11}, promises to reveal a number of new lowdensity superconductors. In particular, perovskites BaTiO_{3} and KTaO_{3} can be tuned to ferroelectric QCPs by pressure^{47} and strain^{48}, respectively, and become metallic under doping^{32,49,50}. Additionally, twodimensional systems created from these materials, such as LaAlO_{3}/SrTiO_{3} interfaces^{51} and surfaces of KTaO_{3}^{52} crystals have been shown to exhibit superconductivity. In the former case, the doping dependence and maximal value of T_{c} suggest that the pairing is driven by the same mechanism as in bulk SrTiO_{3}^{53}. Also, a recently discovered intrinsic polar metal LiOsO_{3}^{54} has been predicted to host nodal points close to the Fermi level (which suggests that small Fermi surfaces with dilute concentrations can be present or created by doping)^{55} and to have a straintuned polar QCP^{56}. In all of these cases, the role of energy fluctuation mechanism in pairing can be verified by the characteristic dependence of the phonon energy on electron concentration (Eq. (6)), scaling of T_{c} with phonon energy (Eq. (17)), and the presence of a related T^{2} component in resistivity at low densities^{28,29}. At the same time, unlike typical scenarios of quantum critical pairing^{57}, the normal state is expected to be a Fermi liquid.
Intriguingly, the “dark matter” scenario identified here in polar metals indeed has a counterpart in the fermionic superfluid scenarios of cosmological dark matter^{58,59}, suggesting that quantum critical polar metals may provide a solidstate platform to study these proposals experimentally. In a broader context, energy fluctuations are ubiquitous at quantum critical points, and may thus play a role in electron pairing in many settings. One instance is the case of superconductivity occurring close to a nonpolar structural transition, driven by a phonon at a highsymmetry point, exemplified by tungsten bronze^{60,61,62} and the A15 compounds^{63}. As in a polar metal, the critical phonon decouples from electrons at low momenta, raising the intriguing possibility of energyfluctuation pairing. Energy fluctuations have been also proposed as alternative drivers of pairing near antiferromagnetic quantum critical points in strongly correlated metals^{64,65}. Finally, the phenomenon of superconductivity mediated by energydensity fluctuations can also serve as a tool to probe “dark matter" aspects of the solid state, involving excitations that do not interact electromagnetically, such as those related to complex hidden orders^{66}.
Note Added: While this work has been under review, Ref. 67 appeared, where a similar mechanism has been applied to SrTiO_{3} at n_{e} ≲ 10^{18} cm^{−3}.
Data availability
All data needed to evaluate the conclusions in the paper are present in the paper and/or the Supplementary Information. Additional data related to this paper may be requested from the authors.
References
Schrieffer, J. Theory of Superconductivity, 3rd edn. (Benjamin/Cummings, Reading MA, 1983).
Bogoljubov, N. N., Tolmachov, V. V. & Širkov, D. V. A new method in the theory of superconductivity. Fortschritte der Physik 6, 605 (1958).
Morel, P. & Anderson, P. W. Calculation of the superconducting state parameters with retarded electronphonon interaction. Phys. Rev. 125, 1263 (1962).
Gurevich, V. Larkin, A. & Firsov, Y. A. Possibility of superconductivity in semiconductors. Sov. Phys.Solid State (Engl. Transl.) (United States) 4, 131 (1962).
Collignon, C., Lin, X., Rischau, C. W., Fauque, B. & Behnia, K. Metallicity and superconductivity in doped strontium titanate. Ann. Rev. Condensed Matter Phys. 10, 25 (2019).
Lin, X., Rischau, C. W., van der Beek, C. J., Fauqué, B. & Behnia, K. swave superconductivity in optimally doped SrTi_{1−x}Nb_{x}O_{3} unveiled by electron irradiation. Phys. Rev. B 92, 174504 (2015).
Swartz, A. G. et al. Polaronic behavior in a weakcoupling superconductor. Proc. Natl. Acad. Sci. 115, 1475 (2018).
Gor’kov, L. P. Phonon mechanism in the most dilute superconductor ntype SrTiO_{3}. Proc. Natl. Acad. Sci. 113, 4646 (2016).
Takada, Y. Theory of Superconductivity in Polar Semiconductors and Its Application to NType Semiconducting SrTiO3. J. Phys. Soc. Japan 49, 1267 (1980).
Ruhman, J. & Lee, P. A. Superconductivity at very low density: The case of strontium titanate. Phys. Rev. B 94, 224515 (2016).
Enderlein, C. et al. Superconductivity mediated by polar modes in ferroelectric metals. Nat. Commun. 11, 4852 (2020).
Ma, J., Yang, R. & Chen, H. A large modulation of electronphonon coupling and an emergent superconducting dome in doped strong ferroelectrics. Nat. Commun. 12, 2314 (2021).
Edge, J. M., Kedem, Y., Aschauer, U., Spaldin, N. A. & Balatsky, A. V. Quantum Critical Origin of the Superconducting Dome in SrTiO_{3}. Phys. Rev. Lett. 115, 247002 (2015).
Stucky, A. et al. Isotope effect in superconducting ndoped SrTiO_{3}. Sci. Rep. 6, 37582 (2016).
Rischau, C. W. et al. A ferroelectric quantum phase transition inside the superconducting dome of Sr_{1−x}Ca_{x}TiO_{3−δ}. Nat. Phys. 13, 643 (2017).
Tomioka, Y., Shirakawa, N., Shibuya, K. & Inoue, I. H. Enhanced superconductivity close to a nonmagnetic quantum critical point in electrondoped strontium titanate. Nat. Commun. 10, 738 (2019).
Wölfle, P. & Balatsky, A. V. Superconductivity at low density near a ferroelectric quantum critical point: Doped SrTiO_{3}. Phys. Rev. B 98, 104505 (2018).
Ruhman, J. & Lee, P. A. Comment on “Superconductivity at low density near a ferroelectric quantum critical point: Doped SrTiO_{3}”. Phys. Rev. B 100, 226501 (2019).
Wölfle, P. & Balatsky, A. V. Reply to “Comment on ‘Superconductivity at low density near a ferroelectric quantum critical point: Doped SrTiO_{3}”’. Phys. Rev. B 100, 226502 (2019).
Kanasugi, S. & Yanase, Y. Spinorbitcoupled ferroelectric superconductivity. Phys. Rev. B 98, 024521 (2018).
Gastiasoro, M. N., Trevisan, T. V. & Fernandes, R. M. Anisotropic superconductivity mediated by ferroelectric fluctuations in cubic systems with spinorbit coupling. Phys. Rev. B 101, 174501 (2020).
Kanasugi, S., Kuzmanovski, D., Balatsky, A. V. & Yanase, Y. Ferroelectricityinduced multiorbital oddfrequency superconductivity in SrTiO_{3}. Phys. Rev. B 102, 184506 (2020).
Kozii, V., Bi, Z. & Ruhman, J. Superconductivity near a ferroelectric quantum critical point in ultralowdensity dirac materials. Phys. Rev. X 9, 031046 (2019).
Volkov, P. A. & Chandra, P. Multiband quantum criticality of polar metals. Phys. Rev. Lett. 124, 237601 (2020).
Fal’ko, V. I. & Narozhny, B. N. Triplet pairing due to spinorbitassisted electronphonon coupling. Phys. Rev. B 74, 012501 (2006).
Kozii, V. & Fu, L. Oddparity superconductivity in the vicinity of inversion symmetry breaking in spinorbitcoupled systems. Phys. Rev. Lett. 115, 207002 (2015).
Ngai, K. L. Twophonon deformation potential and superconductivity in degenerate semiconductors. Phys. Rev. Lett. 32, 215 (1974).
Epifanov, Y. N., Levanyuk, A. P. & Levanyuk, G. M. Interaction of carriers with tophonons and electrical conductivity of ferroelectrics. Ferroelectrics 35, 199 (1981).
Kumar, A., Yudson, V. I. & Maslov, D. L. Quasiparticle and nonquasiparticle transport in doped quantum paraelectrics. Phys. Rev. Lett. 126, 076601 (2021).
Nazaryan, K. G. & Feigel’man, M. V. Conductivity and thermoelectric coefficients of doped SrTiO_{3} at high temperatures. Phys. Rev. B 104, 115201 (2021).
van der Marel, D., Barantani, F. & Rischau, C. W. Possible mechanism for superconductivity in doped SrTiO_{3}. Phys. Rev. Res. 1, 013003 (2019).
Kolodiazhnyi, T., Tachibana, M., Kawaji, H., Hwang, J. & TakayamaMuromachi, E. Persistence of Ferroelectricity in BaTiO_{3} through the InsulatorMetal Transition. Phys. Rev. Lett. 104, 147602 (2010).
Sachdev, S. Quantum Phase Transitions (Cambridge Universtity Press, 1999).
Goldenfeld, N. Lectures on phase transitions and the renormalization group (1992).
Gor’kov, L. P. & MelikBarkhudarov, T. K. Contribution to the theory of superconductivity in an imperfect fermi gas, Soviet Physics JETP 13, 1081 (1961).
Gor’kov, L. P. Superconducting transition temperature: Interacting fermi gas and phonon mechanisms in the nonadiabatic regime. Phys. Rev. B 93, 054517 (2016).
Kleinert, H. & Schakel, A. M. J. GaugeInvariant Critical Exponents for the GinzburgLandau Model. Phys. Rev. Lett. 90, 097001 (2003).
Bäuerle, D., Wagner, D., Wöhlecke, M., Dorner, B. & Kraxenberger, H. Soft modes in semiconducting srtio3: Ii. the ferroelectric mode. Zeitschrift für Physik B Condensed Matter 38, 335 (1980).
Collignon, C. et al. Superfluid density and carrier concentration across a superconducting dome: The case of strontium titanate. Phys. Rev. B 96, 224506 (2017).
Koonce, C. S., Cohen, M. L., Schooley, J. F., Hosler, W. R. & Pfeiffer, E. R. Superconducting Transition Temperatures of Semiconducting SrTiO_{3}. Phys. Rev. 163, 380 (1967).
Lin, X. et al. Critical Doping for the Onset of a TwoBand Superconducting Ground State in SrTiO_{3−δ}. Phys. Rev. Lett. 112, 207002 (2014).
BretzSullivanet, T. M. et al. Superconductivity in the dilute single band limit in reduced strontium titanate (2019), https://arxiv.org/abs/1904.03121.
Gastiasoro, M. N., Ruhman, J. & Fernandes, R. M. Superconductivity in dilute SrTiO_{3}: A review. Ann. Phys. 417, 168107 (2020).
Ahadiet, K., et al. Enhancing superconductivity in SrTiO_{3} films with strain. Sci. Adv. 5, aaw0120 (2019)
Herrera, C. et al. Strainengineered interaction of quantum polar and superconducting phases. Phys. Rev. Materials 3, 124801 (2019).
Zhou, W. & Ariando, A. Review on ferroelectric/polar metals. Japanese J. Appl. Phys. 59, SI0802 (2020).
Ishidate, T., Abe, S., Takahashi, H. & Môri, N. Phase Diagram of BaTiO_{3}. Phys. Rev. Lett. 78, 2397 (1997).
Skoromets, V. et al. Ferroelectric phase transition in polycrystalline KTaO_{3} thin film revealed by terahertz spectroscopy. Appl. Phys. Lett. 99, 052908 (2011).
Sakai, A., Kanno, T., Yotsuhashi, S., Adachi, H. & Tokura, Y. Thermoelectric Properties of ElectronDoped KTaO_{3}. Japanese J. Appl. Phys. 48, 097002 (2009).
Ueno, K. et al. Discovery of superconductivity in KTaO_{3} by electrostatic carrier doping. Nat. Nanotechnol. 6, 408 (2011).
Gariglio, S., Gabay, M. & Triscone, J.M. Research Update: Conductivity and beyond at the LaAlO_{3}/SrTiO_{3} interface. APL Mater. 4, 060701 (2016).
Liu, C. et al. Twodimensional superconductivity and anisotropic transport at KTaO_{3} (111) interfaces. Science 371, 716 (2021).
Valentinis, D. et al. Modulation of the superconducting critical temperature due to quantum confinement at the LaAlO_{3}/SrTiO_{3} interface. Phys. Rev. B 96, 094518 (2017).
Shi, Y. et al. A ferroelectriclike structural transition in a metal. Nat. Mater. 12, 1024 (2013).
Yu, W. C. et al. Nonsymmorphic cubic Dirac point and crossed nodal rings across the ferroelectric phase transition in LiOsO_{3}. Phys. Rev. Materials 2, 051201 (2018).
Narayan, A. Effect of strain and doping on the polar metal phase in LiOsO3. J. Phys. Condensed Matter 32, 125501 (2019).
Chubukov, A. V., Abanov, A., Wang, Y. & Wu, Y.M. The interplay between superconductivity and nonfermi liquid at a quantumcritical point in a metal. Ann. Phys. 417, 168142 (2020).
S., Alexander, S., & Cormack, S. Gravitationally bound BCS state as dark matter. J. Cosmol. Astropart. Phys. 2017, 005 (2017)
Alexander, S., McDonough, E., & Spergel, D. N. Chiral gravitational waves and baryon superfluid dark matter. J. Cosmol. Astropart. Phys. 2018, JCAP05 (2018)
Raub, C. J., Sweedler, A. R., Jensen, M. A., Broadston, S. & Matthias, B. T. Superconductivity of sodium tungsten bronzes. Phys. Rev. Lett. 13, 746 (1964).
Pellegrini, C., Glawe, H. & Sanna, A. Density functional theory of superconductivity in doped tungsten oxides. Phys. Rev. Materials 3, 064804 (2019).
Mascello, N., Spaldin, N. A., Narayan, A. & Meier, Q. N. Theoretical investigation of twin boundaries in WO_{3}: Structure, properties, and implications for superconductivity. Phys. Rev. Research 2, 033460 (2020).
Stewart, G. Superconductivity in the a15 structure. Physica C: Supercond Appl. 514, 28 (2015).
Abrahams, E., Schmalian, J. & Wölfle, P. Strongcoupling theory of heavyfermion criticality. Phys. Rev. B 90, 045105 (2014).
Kang, J., Fernandes, R. M., Abrahams, E. & Wölfle, P. Superconductivity at an antiferromagnetic quantum critical point: Role of energy fluctuations. Phys. Rev. B 98, 214515 (2018).
Aeppli, G., Balatsky, A. V., Rønnow, H. M. & Spaldin, N. A. Hidden, entangled and resonating order. Nat. Rev. Mater. 5, 477 (2020).
Kiselov, D. E. & Feigel’man, M. V. Theory of superconductivity due to Ngai’s mechanism in lightly doped SrTiO_{3}. Phys. Rev. B 104, L220506 (2021).
Acknowledgements
The authors gratefully acknowledge stimulating discussions with D. L. Maslov, and with the late P. W. Anderson during early stages of this work. P. A. V. is supported by a Rutgers Center for Materials Theory Abrahams Fellowship, P. Chandra is supported by DOE Basic Energy Sciences grant DESC0020353 and P. Coleman is supported by NSF grant DMR1830707.
Author information
Authors and Affiliations
Contributions
P.A.V. contributed to formulating the problem, performed the analytical and numerical calculations and contributed to analyzing the results and writing the manuscript. P. Chandra contributed to formulating the problem, analyzing the results and writing the manuscript. P. Coleman contributed to formulating the problem, analyzing the results and writing the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Peer review
Peer review information
Nature Communications thanks Hanghui Chen and the other, anonymous, reviewer(s) for their contribution to the peer review of this work. Peer reviewer reports are available.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Volkov, P.A., Chandra, P. & Coleman, P. Superconductivity from energy fluctuations in dilute quantum critical polar metals. Nat Commun 13, 4599 (2022). https://doi.org/10.1038/s41467022323032
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467022323032
This article is cited by

Phononmediated spin transport in quantum paraelectric metals
npj Quantum Materials (2024)

Stoichiometric control of electron mobility and 2D superconductivity at LaAlO3SrTiO3 interfaces
Communications Physics (2024)

Superconductivity enhancement in polar metal regions of Sr0.95Ba0.05TiO3 and Sr0.985Ca0.015TiO3 revealed by systematic Nb doping
npj Quantum Materials (2022)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.